# uncasi ad-a230 a -at8 · uncasi ad-a230 2a. security ... in this report we focus on polymer welding...

Post on 29-Jul-2018

219 views

Embed Size (px)

TRANSCRIPT

UNCLASSIFIED MASTER COPY t FOR REPRODUCTION PURPOSFSECURITY CLASSIFICATION OF THIS PAGE

REPORT Ila. REPORT SECURITY CLASSIFICATION

Uncasi AD-A2302a. SECURITY CLASSIFICATION AUTHORITY A -AT82b. DECLASSIFICATIONiDOWNGRADING SCHEDUL- Approved for public release, A.ji

distribution unlimited.4. PERFORMING ORGANIZATION REPORT NUMBER(S) S. MONITORING ORGANIZATION REPORT NU ER(

6a. NAME OF PERFORMING ORGANIZATION 6b. OFFICE SYMBOL 7a. NAME OF MONITORING ORGANIZATION J(If applicable,

UNIVERSITY OF ILLINOIS U. S. Army Research Office

6c. ADDRESS (City, State, and ZIP Code) 7b. ADDRESS (City, State, and ZIP Code)

P. 0. Box 12211URBANA IL 61801 Research Triangle Park, NC 27709-2211

8a. NAME OF FUNDING /SPONSORING 8b. OFFICE SYMBOL 9. PROCUREMENT INSTRUMENT IDENTIFICATION NUMBERORGANIZATION (If applicable)

U. S. Army Research Office -Df:fIL.S0 3 6-k-O 018c. A, (RESS (City State. and ZIP Code) 10. SOURCE OF FUNDING NUMBERS

P. 0. Box 12211 PROGRAM PROJECT TASK WORK UNITELEMENT NO. NO. NO. ACCESSION NO

Re-:Pdrch Triangle Park, NC 27709-2211

11. TITLE (Include Security Classification)

STRENGTH OF POLYMER INTERFACES

12. PERSONAL AUTHOR(S)R. P. WOOL

13a. TYPE OF REPORT "13b. TIME COVERED 14. DATE OF REPORT (Year, Month, Day)111,5 PAGE COUNTFINAL I FROM 1/86 TO 1/89 I 90/11/25 I

1'6. SUPPLEMENTARY' NOTATION ..The view, opinions and/or findings contained in this report are those

of the authr($).and sh uld not be construed as an fficial Department of the Army position,

17. COSATI CODES 18. SUBJECT TERMS (Continue on reverse if necessary and identify by block number)

FIELD GROUP SUB-GROUP 1110 POLYMER WELDING, INTERFACE STRUCTURE, FRACTURE, FATIGUE,

LAMINATION, DIFFUSION r c.~wC~&La 1 ~19. ABSTRACT (Continue on reverse if necessary and identify by block numbe.)

"- Studies df strength development at polymer-polymer interfaces are examined and applicaticns towelding of simil~r and dissimilar polymers are considered. The fracture properties of the weld, namely,fracture stress, 6, fracture energy, GIc, fatigue crack propagation rate da/dN, and microscopic aspects ofthe deformation process are determined using compact tension, wedge cleavage, and double cantileverbeam healing experiments. The mechanical properties are related to the structure of the interface viamicroscopic deformation mechanisms involving disentanglement and bond rupture. The time dependentstructure of the welding interface is determined in terms of the molecular dynamics of the polymerchains, the chemical compatibility, and the fractal nature of diffuse interfaces. Several experimentalmethods are used to probe the weld structure and compare with theoretical scaling laws. Results aregiven for symmetric amorphous welds, incompatible and compatible asymmetric amorphous welds,incompatible semicrystalline and polymer-metal welds. The relevance of interface healing studies tothermal, friction, solvent and ultrasonic welds is discussed.

20. DISTRIBUTION /AVAILABILITY OF ABSTRACT 21, ABSTRACT SECURITY CLASSIFICATION

I]UNCLASSIFIEDAJNLIMITED 0 SAME AS RPT. - DTIC USERS Unclassified22a. NAME OF RESPONSIBLE INDIVIDUAL 122b. TELEPHONE (inciude Are. Code} Uc. OfFiCE SMBOL

RICHARD P. WOOL (217) 333-2468

DO FORM 1473,84 MAR 83 APR edition may be used until exhausted SECURITY CLASSIFICATION OF THIS PAGEAll other editions are obsolete UNCIASSIFTED

UNIS 9 TE

STRENGTH OF POLYMER INTERFACES

by

Richard P. Wool

(217) 222-2468

Department of Materials Science and EngineeringUniversity of Illinois, 1304 W. Green St., Urbana, Illinois 61801

Final Report, Proposal No. 22966-MSArmy Research Office, Durham, NC

Version 4.0

Nov., 1990

3

ABSTRACT

Studies of strength development at polymer-polymer interfaces are examined andapplications to welding of similar and dissimilar polymers are considered. The fractureproperties of the weld, namely, fracture stress, or, fracture energy, GIc, fatigue crackpropagation rate da/dN, and microscopic aspects of the deformation process aredetermined using compact tension, wedge cleavage, and double cantilever beam healingexperiments. The mechanical properties are related to the structure of the interface viamicroscopic deformation mechanisms involving disentanglement and bond rupture. Thetime dependent structure of the welding interface is determined in terms of the moleculardynamics of the polymer chains, the chemical compatibility, and the fractal nature ofdiffuse interfaces. Several experimental methods are used to probe the weld structure andcompare with theoretical scaling laws. Results are given for symmetric amorphous welds,incompatible and compatible asymmetric amorphous welds, incompatible semicrystallineand polymer-metal welds. The relevance of interface healing studies to thermal, friction,solvent and ultrasonic welds is discussed.

Accession For

NTIS GRA&I

DTIC TAB

Unannou--ced Ljustificatio

By-

Distribution/ _

Avalability Codes

Avail and/orDist Speci a l

10

4

INTRODUCTION

The joining or welding of polymers can be accomplished by several techniquesinvolving thermal welding, vibrational welding, friction welding, solvent welding, surfacechemical modification, ion beam surface modification, resonance heating and other moreexotic but less common techniques. In this Report we focus on polymer welding where themolecules near the surfaces become mobile and the weld strength develops by a combin-ation of surface rearrangement, wetting and diffusion. The molecular mobility can beinduced by heat from friction, (ultrasonic) vibration, impact, hot plates, solvents, etc.

In recent years, we have considered the problem of strength development at polymer-polymer interfaces in terms of the static and dynamic properties of random-coil chains (1-4). When two pieces of molten polymer are brought into contact, wetting or closemolecular contact (van der Waals) first occurs followed by interdiffusion of chain segmentsback and forth across the wetted interface. After a contact time, t, we inquire as to themechanical energy, G, required to separate the two pieces as a function of time, temper-ature, T, contact pressure, P, and molecular weight, M, of the linear random-coil chains,i.e.,

G = W(t, T, P, M) (1)where W is the welding function to be determined. Solutions to -his problem haveapplication to similar situations involving polymer-polymer interfaces. For example,processing of powder and pellet resin, internal weld lines of polymer melts during extrusionand injection molding, welding of surfaces, lamination of composites, coextrusion, andautohesion of uncured linear elastomers.

In this Report, we focus on problems of welding and autohesion with emphasis onsymmetric interfaces where the same amorphous polymer exists on both sides of theinterface. Consideration is also given to the important case of incompatible asymmetricamorphous and crystalline interfaces where strength develops between two immisciblepolymers. We begin by introducing the reptation model (5, 6) for diffusion at a symmetricinterface and determlne a molecular description of the interface structure as a function ofthe variables, t, T, P, and M. We then discuss models to relate the interface structure tothe mechanical properties via a set of microscopic deformation mechanisms. The latterinvolve disentanglement by chain pullout, bond rupture and connectivity between chains.The predictions for welding, tack and green strength are compared with experiments andtheories (7-11) of other investigators.

5

THEORY

Molecular Dynamics of Random-Coil Chains

The motion of individual chains in amorphous bulk materials or concentrated solutionsof linear random-coil (Gaussian) chains has been modelled by the reptation theory of deGennes (5) and Edwards (6). In this model the chain is confined to a tube having a similarshape as the random-coil configuration of the chain. The tube represents topologicalconstraints to la: ral motion of monomers imposed by the neighboring chains via entangle-ments and predt ninantly restricts motion of the chain to that along the curvilinear lengthof the tube. Our use of this model is illustrated in Fig. 1. At t = 0, the chain (solid line) isin its initial tube indicated by the dashed lines. The chain exhibits Brownian motion backand forth in the tube and because the chain ends are free to move in any direction awayfrom the tube, the memory of the initial tube position in space is gradually lost as shown attimes t2 and t3. However, the chain being in a dense system is always in a new tube butonly parts of the chain, usually towards the center, retain memory of the initial tube for therelaxation time, Tr. The length of chain, 1(t), which "escapes" from the initial tube is also arandom-coil chain obeying Gaussian statistics and we call it the minor chain (2). As theminor chain increases in length we can represent its static dimensions by a "most probable"spherical envelope as shown in Fig. 1.

MINORCHAIN

Sj CHAIN

Ito

MINOR MINOR' CHAIN C

H A IN

t-t2 Tr

0

6

DI -_ M 1. (3)The mean square monomer displacement of the minor chains:

= 1/2. (4)The mean square center-of-mass diffusion distance, < X 2cm >:

= 2Dt. (5)The center-of-mass self-diffusion coefficient, D:

D = M -2 (6)The reptation time, Tr:

Tr = M 3 (7)The fraction of chain remaining in the tube, F(t):

F(t) = 1 - 4/73/ 2 (t/Tr)1 / 2 , (8)where t < Tr.For t > Tr, F(t) can be well approximated by (5, 12),

F(t) :% 8/;r2e't/Tr. (9)

Equations 8 and 9 form the basis for describing the viscoelastic shear relaxationmodulus of the Doi-Edwards(12) constitutive theory of entangled linear polymer melts.Considerable experimental support exists for the molecular weight dependence of the self-diffusion coefficient, Eq. 5, and has been reviewed by Tirrell (13). Support for the minorchain model shown in Fig. 1 has recently been obtained by Lee and Wool and by Walczakand Wool (14). Using FTIR techniques, they showed that the orientation relaxation ofstep-strained centrally deuteriated polystyrene chains first occurred by relaxation of theprotonated chain ends while the center of the chain retained its orientation. The chainswere diluted in a higher molecular weight matrix. The centrally deuteriated part of thetriblock chain then relaxed at a predicted time and rate consistent with the reptationtheory. The homopolymer chains (without the higher molecular weight matrix) do notshow this effect which we believe is due to the percolation relaxation mechanism recentlyproposed by us. However, the reptation theory fails to accurately predict the molecularweight dependence of thf zero-shear viscosity with a 3.4 power law exponent. Therelaxation time, Tr = M', is also important in determining healing or welding times atpolymer interfaces. In the next section we use the minor chain model to develop a timeand molecular weight dependent molecular description of a polymer interface. Effects oftemperature and pressure will also be discussed.

Molecular Description of a Polymer-Polymer Interface

The most important interface to consider is that formed by a symmetric A/A polymerpair consisting of linear monodisperse molecular weight polymers whose chain ends areuniformly distributed in the bulk melt material. Polydisperse symmetric A/A pairs andsome asymmetric A/B pairs can also be investigated using methods presented in thissection. Assuming instantaneous wetting (time-dependent wetting is considered later) ofthe two surfaces we proceed to analyze the molecular aspects of the interface arising frominterdiffusion. This problem is simplified further using the minor chain model as shown inFig. 2.

(o) 7INTERFACE MMINOR

CHAINC~)SGMEfNT

=0 l=I

t' '2

(b)0< t' < t2< Tr

0

0oQ

Fig. 2. The interdiffusion process at a polymer-polymer interface in terms of the behaviorof (a) the minor chains and (b) the minor chain spherical envelopes. Only one side of theinterface is shown for convenience. Instantaneous molecular contact or wetting is assumedat t = 0 (Kim and Wool).

At t = 0, molecular contact is achieved at the interface (only the molecules on one sideof the interface are shown for clarity). The chains begin to reptate via their chain endswhich are shown initially as dots randomly distributed in space. As time proceeds, only thatpart of the chain which has escaped its original configuration, i.e., the minor chain, cancontribute to interdiffusion across the interface. Furthermore, we do not have to considerthe exact location of each segment of the minor chain but only the spherical envelope towhich it belongs, as shown in Fig. 2. Thus, as time approaches the reptation time, Tr, inter-penetration and reentanglement of chains are achieved and the molecular properties of thevirgin state are obtained at the interface plane. From this minor chain model, manymolecular aspects of the interdiffusion process can be determined, as presented below.Solutions are given for t < Tr (healing) and t > Tr (virgin state). Details of thecalculations are given in references 2, 3, and 15.

Number of Chains Intersecting the Interface, n(t)

The number of random-coil chains intersecting unit area of the interface as a functionof contact time, t, and molecular weight, M, behaves as,

n(t) = t1 / 4 M-5 / 4 ; (t < Tr) (10)

nco = M- 1/ 2 . (t > Tr) (11)A chain is considered to intersect the interface when one of its ends has crossed theinterface contact plane defined at t = 0. n(t) also scales as X/M where X is the averagemonomer segment interpenetration distance defined by Eq. 4. Eq. 10 is derived on thebasis that all chains whose ends are within a distance of Xfrom the interface will haveintersected the interface at time t, and thai Ue number of h ns per unit volume varies asM' . The time-dependence is a typically t rather than t as expected for usual atomicdiffusion processes.

Note that the staticyr virgin state solution at t > Tr is obtained by substituting for thereptation time, Tr = M in the dynamic solution. The static solutions are independent ofthe molecular dynamics model and can be derived from other considerations. Eq. 11 wasderived previously by Wool and Rockhill (17). Thus, the dynamic solutions give the staticsolutions simply by substituting for the molecular weight dependence of the relaxation

8

time. This is an important feature in evaluating molecular aspects of strengthdcvelopment.

When a molecular property is suggested as controlling the time dependence of welding,that property can be used to simultaneously predict both the molecular weight dependenceof welding and the molecular weight dependence of fracture in the virgin state. This threeway concurrence is useful in evaluating potential solutions to welding problems. Forexample, it is known from the experiments of Kausch, et al. (18-20) and Wool, fe4al. (1, 21,22) that the fracture stress during crack healing and welding increases as o = t / . It couldbe hypothesized up[p inspection of Eq. 10 that the number of chains intersectin theinterface, n(t) , is responsible for the strength development. However, thishypothesis can be rejected by examining the virgin state property, Eq. 11, since the frcturestress of polymers does not decrease with increasing molecular weight as a.o M-1-Further experimental study would show that the healing rate does not depend on M- 5 / 4 .Conversely, molecular properties used to describe the virgin state strength can also beevaluated by their ability to describe the time and molecular weight dependence of healing.This argument applies when the same microscopic deformation mechanisms are operativeduring welding and fracture of the virgin state.

Average Interpenetration Contour Length, 1(t)

The average contour length of chain segments or cilia which have diffused across theinterface is obtained from the minor chain model as,

l(t) t1/2 M-1 / 2 (12)

l , M (13)This property has the same scaling relation as the minor chain length, < 1 >. It will beshown later that l(t) is important in determining mechanical properties wheredisentanglement and chain pullout are dominant microscopic deformation mechanisms.

Number of Bridges Crossing Interface, p(t)

Each time a piece of interdiffusing chain crosses back and forth through the interface,it creates a molecular bridge. Intuitively, this may be visualized as a "sewing up" of theinterface. p(t) is determined by p(t) = n(t)vl(t) where v'l(t) is proportional to the numberof bridges created by each minor chain (a random walk of N steps originating at a planewill cross the plane VN times). Thus we obtain,

p(t) - t 1 / 2 M-3 / 2 (14)

PCO MO. (15)This result was first obtained by de Gennes (9) using a scaling law and is equivalent to

the "crossing density" determined by Prager and Tirrell (7) from a more detailed calcula-tion of the interdiffusion process. Note that the virgin state number of bridges isindependent of molecular weight. Thus, bridges alone cannot be used to describe strengthdevelopment during welding in cases where the virgin strength exhibits a molecular weightdependence over some range of molecular weight as observed for most polymers.

Modifications to the bridge models have been suggested by Adolf Tirrell and Prager (7)and later by Mikos and Papas (29) which involve a minimum interpenetration depth, Xe, todevelop entanglements. These approaches introduced a molecular weight dependence for

9

the virgin state, resolving the problem posed by Eq. 15 and gave a more complex expressionfoi he time depe.dence of heahing. Extrapolation of long time healing data to zerostrength is predicted by this modification to intersect tbh time axis at a finite time, t.,required to diffuse to the minimum distance Xe. This effect has not been observed in manywelding studies conducted by various groups.

Polydispersity effects were also considered by Adolf, Tirrell and Prager (7). Assumingindependent reptating chain diffusion, the contribution to the concentration profile fromindividual chains can be readily determined for any molecular weight distribution. At shorttimes, the contribution from the faster diffusing shorter chains dominates the weld strengthfollowed later by the slower diffusing longer chains. This can result in highly nonlinea-welding behavior as demonstrated by McGarel and Wool (54) for welding of polystyrene.Bridge concepts are also useful in the development of entanglement models and forestimating the number of broken bonds in brittle fracture.

Average Monomer Interpenetration Depth, X(t)

The average monomer interpenetration depth of segments on the interdiffusing chains,X(t), is obtained from an integration over the Gaussian segment density profiles of theinterdiffused minor chain population, (2) as shown in Fig. 3, such that,

X(t) M (16)

X,, M1/2_= R/V6 (17)

At t = Tr, the average monqr r interpenetration distance is equal to the radius ofgyration, or X. =R/N/6. The t'q dependence in Eq. 16 is unique to the correlated motionof the chains for times less than the reptation time. This result can be understood by

p

IIII

I y=O Y=yO y AXIS

- x

Fig. 3. Segment density, p, of minor chains and the average interpenetration distance, x(Kim and Wool).

considering the Brownian rqojon and displacement, s, of an individual monomer along thecontour of the tube as s = t'/ f t < Tr.However, the curvilinear motion is related totranslational motion via X = sl because the chain is a random-coil. For times greaterthan Tr, when the original tube has evaporated the motion of the monomer becomesuncorrelated since s is greater than the chain length and its displacement becomes similarto the center-of-mass displacement, Xcm,

Xcm : tl/2M -1 (18)

1 0

The crossover from t1 /14 to t1 / 2 behavior could be examined by fexperimentaltechniques such as Secondary Ion Mass Spectrometry (SIMS), Sputtered Neutral AtomMass spectrometry (SNMS), (23) and Neutron Specular Reflectivity (NSR), which probethe concentration profile at a polymer interface for t < T and distances X < R . Centerof mass motion for t > Tr and X R is well established from self-diffusion studies andfound to be in agreementI/4tn Eq. 18. For chains in the bilk, the monomer rp$i,on ispredicted to proceed as t /for t < T r while the center-of-mass proceeds as t/L at alltimes. Doi and Edwards (12) showed that the center-of-mass motion is uncorrelated at alltimes by virtue of the random motion of the chain ends.

Eq. 18 cannot be used to describe center-of-mass motion for chains whose random-coilconfigurations o.e altered by the interface as shown in Fig. 4. The chains initially have anon-Gaussian configuration due to the reflecting boundary condition at the surface. As theminor chains interdiffuse, the configurations of the affected chains in the surface layer relaxto Gaussian configurations. In Fig. 4, the average shape and size of a chain at the interface(solid vertical line) before and after relaxation are shown. The distance, ?7, from thelocation of the highest segment density of the chain to the interface remains constantduring the relaxation. Since the center-of-mass of each chain is close to the peak of thesegment density profile, it can be seen that vry little motion of the center-ot-mass occursfor t < Tr . For a chain in the bulk, the center-of-mass is displaced by a distance approxi-mately equal to its end-to-end vector, R, during 1,e same relaxation time. Since R > r, the"apparent center-of-mass self-diffusion coefficient" of chains affected by the interfacewould be smaller than that of chains further away from the interface in the bulk. Thisargument underlies the qualification for the center-of-mass scaling law in Table 1.

The nonequilibrium configurations of the chains near the interface plays an importantrole in deterrmning entanglement density and the structure of asymmetric incompatibleamorphous interfaces. The reduced entropy of the confined chain configurations shown inFig. 4 acts as a driving force to achieve limited diffusion in the interface of immisciblepolymers. The increase in entropy is counterbalanced by a positive enthalpy of rnig andresults in an equilibrium thickness predicted by Helfand, et al. (24) as d", Chi whereChi is the Flory-Huggins interaction parameter (25).

t0)

INTERFACE

I NON-GAUSSIAN

GAUSSIAN

77l 77I1=

(b)

p p

r NON -GAUSSIAN

G SIAN

21 , I-1:O I >Tr

Fig. 4. (a) Average shape and size of a zhain at the interface before and after healing. (b)Segment density, V, of the chain in (a) before and after healing (Kim and Wool).

Namber cf Monomers Crossing Interface, Lo(t)

Tl9e number of monomers which have crossed from one side of the interface to theother is equivalent to the total interpenetration contour length, Lo(t) = n(t)l(t). Summingover the segment density profiles of the interdiffused minor chains, we obtain, (15)

Lo(t) t3 / 4 N- 7 / 4 ; (19)

L MV M 2. (20)The i/risual t3 / 4 dependence s again due to correlated motion effects and reverts to a

normal tlL diffusion-dependence for times greater than Tr. This result has beensupported by experimerpal techniques discussed in reference 23 where Lo is determinedfrom the integral of the concentration profile.

Concentration Profile

Integrating over the population of interdiffused minor chain Gaussian segment densityprofiles shown in Figs. 2 and 3, the normalized monomer concentration profile FD(x,t), forthe symmetric polymer-polymer interface was obtained by Zhang and Wool (15) for t < Tras,

1)(x,t) = [I(t)/L + x2/bL] erfc[x/(b,/2n)] (21)

-V(2n/ar) (x/L) exp [-x2/(2nb2)]

where b is the bond length, n is the number of monomers ii, the minor chain of length 1(t),x is the diffusion depth such that x = 0 at the interface and L is the contour length of theentire chain. The time dependence of the concentration profile in Eq. 21 derives from thetime-dependence of the minor chains via l(t) = V(16 D1 t/.7r).

Computed concentration profiles are shown in Fig. 5 at fractional reptation times anddiffusion depths normalized with respect to the end-to-end vector of the Gaussian chains(15). Fig. 5 clearly shows that the concentration at the initially joined interface at x = 0 isdiscontinuous when the welding time is shorter than the reptation time. For normal

10

0.90.68

0.3

0 50.6- 0.7

0.9

, 0.4- 0.6

0~ 0.4

202

0

-100 -50 0 50 100

ODslonce From Inlerface, x/Rq x 100

Fig. 5. Concentration profile of a polymer-polymer interface at time- t less than thereptation time, Tr. The interdiffusion depth, x, is normalized with respect to the radius ofgyration, Rg (Zhang and Wool).

12

Fickian di,,usion, the atomic or monomer concentration profile at the origin immediatelyattains a value of 0.5, (assuming an initially sharp interface at t = 0) since the Brownianmotion of the atoms is isotropic. For polymers howevei, the majority of monoriers irncontact with the initial plane exhibit anisotropic motion due to their counectivity. '1 hey arenot free to interdiffuse on the time scale of monomer motion but await the diffusicn of themuch smaller number of minor chain ends. Thus, 4F(x,t) contains a discontinuity at x = 0which is an interesting peculiarity of the reptation model and persists for at least onereptation time. The discontinuity or gap na,' be difficult to observe experimentallybecause the short range segmental mot.on may obscure the gap rear x = 0 (i5). However,analysi , of the entire profile shape, particularly at x >> 0, should give crit-"al insight into thereptation model. This work is in progress using Neutron Reflection.

For t > Tr, the con"entration profile returns to the cla:..sical Fickian profile,

FD(x) = erfc(x/Ld), (22)

where Ld is the Einstein diffusion length given by Lc0 = 2Vx(Dt). The non-Fickiancharacteristics of the concentration profile due to correlated motion effects in the reptationmudel have been discussed by de Gennes, (9) Prager and Tir-ell, (28) and by Zhang andWool (15). Eq. 21 has also been used to calculate the molecular properties of the interface

-d these results are summarized in Table 1 (15).

Scaling Laws for a Polymer-I olynxer Interface

The molecular properties described above and others listed in Table 1 have aconvenient common scaling law which relates the dynamic properties, H(t), to the staticproperties, Ho, via the reduced time, t/Tr, by (4)

14"t) Ho,-I (t/Tr )r/4; (23)

I.t M(3r-s)/ 4 (24)

where r, s = 1,2,3 ....

Table 1 summarizes the average dynamic and static molecular properties of a polymer-polymer inteiface and lists values of i and s for indi'vidual properties. This table can beused to detrmne other properties and evaluate sugg.;stions and theories relating interfacestructure to mechanical properties. Several of these properties have also been derived byde Gennes (9, 26, 27) and by Prager and Tirrell (7, 28, 29).

Table 1. Molecular Aspects of fnterdiffusian at a Polymer-Polyme, Interface.

Dynamic Relation Static RelationMolecular Aspect -ymbol H(t) H. r s

Gen( ral proerty H(t) t'14 M -. /4 M 0'- 8" v r sNo. of chains n(t) t 'M 5 1'- M

-Ir2 1 5

No. of bridge p(t) t '12M -3M1 2 6Ave. monomer depth X(t) t 114 M - "/ m V2 1 1Total monomer depth Xot) Irm M-3( MO 2 6Ave contour lengtt, Q(t) t 'r2M -I M 2 2Total contour length, no. of monomers, N L0(t) t314M-714 M ' 3 7Avr bndge length tQ(t) 1"M -' M'1 2 1 1* Center of mass depth Xt,. tf2M-' M 7 ,r 2 5Diffusion frof, 'ngth N, t 'r0M-3/2 '0 2 6 This equeton Sppli to chains In Ihi bulk and do" not sply to chain* wtoa. cent. of mass Is within a radius of gyrtion -f the suife.

13

If a mechanical property such as the fracture energy, G, is controllei y one of theproperties, H(t), then the time-depen ce of welding is given by G = tr/' and themolecular weight dependence by M- /' . Considering the complexity of the fracturemechanics and deformation mechanisms, it may be an overly simplified argument tosuggest that a single molecular property defined typically over a few hundred angstromthickness of the interface is responsible for the energy dissipation and behavior of a muchlarger deformation zone at the crack tip. However, the scaling laws presented in Table 1offer a convenient framework for evaluating molecular models in terms of the static anddynamic properties of the polymer chains.

FRACTAL NATURE OF A DIFFUSION FRONT

Atomic Diffusion Front

While the concentration profile due to diffusion varies smoothly with depth as shown inFig. 5, the diffusion field when viewed in two or three dimensions has a very rough nature.Consider the two-dimensional lattice diffusion of A-atoms (Fig. 6) into B-atoms (notshown) as discussed by Sapoval, et al (30-32). The concentration prafile of A-atoms isgiven by the Fickian result, 4(x) = erfc(x/Ld), where Ld = 2(Dt)'I' is the Einsteindiffusion length at time, t, with diffusion coefficient, D. "The diffusion "front" (heavy line inFig. 6) is defined by those A atoms which are connected to the diffusion source at X = 0via other A atoms and have an empty first or second B neighbor which is itself connected tothe source of B atoms. The interface with a diffusion front is seen to consist of solidregions with lakes or holes leading down to the "seashore" and unconnected islands of Aatoms in the B "sea". The presence of holes and the connectednet oetween atoms in theinterface is important in determining electrical and mechanical pi iperties of the interface.

A Atom

x-iiT7K1 BLattio -

I

I , !T IT 1 7 T 1

tK

7 'iTt, I44- 0

I' -L 'I

Fig. 6. Schematic of a two-dimensional diffusion field at a given time. The heavy linerepresents the "Diffusion Front" determined by the leading edge of A-atoms connected totheir diffusion source at x = 0 and having at least one B-neighbor connected to its source.The position of the center of the front occurs at Xf and the width of the front is 2of (FromSapoval, et al., Reference 30).

Sapoval, et al. (30-32), determined the frontier to have fractal properties involing self-similarity (scale invariance) and incompleteness of space filling (holes). The fractalgeometry of the frontier is determined by the mass to radius relation, (33)

14

M - RDf, (25)where Df is the fractal dimension of the diffusion front. The fractal geometry exists onlyover the width af of the front as shown in Fig. 6. In two dimensions, D = 1.76. Thenumber of particles per unit width of the front, Nf, increases with the diffusion lengthaccording to

Nf = 0.96 Lda, (26)where the exponent a is given by,

a = (Df-1)v/(l+v), (27)in which v = 4/3 is the critical exponent for the percolation coherence length in twodimensions, resulting in a = 0.43. The latter result is also supported by computersimulation studies of Wool and Long (34). The mean poiiLion of the frontier can be shownto occur at a concentration corresponding to the percolation threshold, Pc (30). In twodimensions, pp. = 0.59, such that particles in the profile at D < Pc are not accessible orconnected while particles in the gradient at (D > Pc are connected to the source at x = 0.The three-dimensional analysis of diffusion fronts is more complex (31).

Eq. ?6 4&dicates how the interface "roughness" increases with diffusion length such thatNf Ld ' . Thus, even though the average concentration profile varies smoothly, thediffusion front can have considerable lateral roughness as shown in Fig. 6. Experimentalexamples of this behavior are described in reference 34 based on studies of electrochemicalreduction of metal ions diffusing in polymers by S. Mazur (35). Fig. 7 shows a polymermetal interface produced by electrochemically depositing silver atoms in a polyimide film.

MONOMER INTERFACE

"- , -, " , I

Fig. 7. Computer simulation of -- -:0- rtt- " E(a) monomer interface, (b) polymer- . . , -interface, and (c) the connected .1 .region of a silver/polyimide inter- - ........ -face (Wool and Long). POLYMER INTERFACE

POLYMER-METAL INTERFACE

15

Atoms not in contact with the source (bottom of Fig. 7) were removed from the electronmicro~raph to reveal the highly ramified nature of the interface. The fractal dimension ofthe thinly sliced interface diffusion front was determined to be about 7/4 in agreement withSapoval's theory. Details of this analysis are given in references 34 and 36.

The ability to control the interface roughness and molecular connectivity hasinteresting implications for the mechanical and electrical property development ofinterfaces. Roughness promotes mechanical interlocking but fractal characteristics withholes reduce electrical conductance and affect signal speed in the metal layer. Thethickness of the conducting strip is determined by the position of the fractal diffusion front.The fractal analysis of interfaces has been found useful by us for the examination ofstructure development at reacting polymer-cement interfaces and for investigatin,biodegradation of cemposites containing degradable and non degradable compon.a.ts, e.g.,starch and polyethylene blends. Biodegradation of such blends involves a percolationinvasion process for materials in which the starch molecules are uniformly distributed inthe PE matrix. However, when flow induced concentration profiles develop, the starchnear the surface is removed by microbes while the remaining material is encapsulatedwithin the PE matrix. The surface separating the accessed material from the encapsulatedmaterial is similar to the fractal diffusion front shown in Fig. 7.

Computer Analysis of Polymer-Polymer Interdiffusion

A computer simulation of reptating random-coil chains diffusing on a square latticeacross an interface plane was conducted (34). An IBM-AT microcomputer attached to aCray XMP-48 was used to simulate the Brownian motion of the interpenetrating chains.The object of this study was to (a) investigate the scaling laws derived for polymerinterdiffu ion shown in Table 1, (b) evaluate the non-Fickian concentration profiles forpolymer diffusion at times less than the reptation time, and (c) to examine fractalcharacteristics of polymer diffusion fronts.

Brownian motion was accomplished by an algorithm which randomly chose a chain endand added a new monomer in one of three possible new directions and subtracted amonomer from the other end. The process was then repeated for each chain. The chainend distribution function was chosen to be uniform behind the interface plane. The basicreptation dynamic results were checked for consistency; namely, that (1) the relaxationtime behaved as Tr = M3, (2) the center-of-mass diffusion coefficient behaved as D = M-2, and (3) that the monomer displacement r(t) behaved as,

{ 2}n = tl/2. (tTr) (30)where r(t) is the position vector of the nth monomer at time t. The monomer displacementaverage is determined over all monomers on each chain.

The chain density was chosen to be inversely proportional to the molecular weight andthe monomer density in the virgin state was chosen to consist of an average of fivemonomers per lattice site to account for interpenetration of random-coil chain statisticalsegments.

At t = 0, the reptating chains were allowed to diffuse across the interface plane andformed ramified structures as shown in Fig. 7. The polymer interface is seen to consist offeatures resembling lakes, islands and seashore similar to the previous atomic diffusion

16

case. However, many of the holes near the x = 0 plane are not due to the fractal nature ofdiffusion but rather are due to the monomer correlated motion effect producing disconti-nuities in the interface as shown in Fig. 5. The computer simulation gave further support tothe scaling laws shown in Table 1 and the concentration profile proposed by Zhang andWool, Eq. 21. Fractal properties of polymer interfaces are discussed in the next section.

Fractal Polymer Diffusion Fronts

The analysis of the fractal nature of polymer diffusion fronts (34) is complicated by theinterpenetrated nature of the random-coil chains allowing several statistical segments ormonomers to occupy a single lattice site. Fig. 7 shows a typical ramified diffusion field forthe simtlated interface. The diffusion front was obtained using the same techniqueemployed by Sapoval, et al (30). The front is potentially more ramified initially due to theconnectivity of monomers within a given chain. Fig. 8 shows the number of monomer onthe diffusion front, Nm, as a function of the average interdiffusion distance, < X >, forrandom-coil chains of molecular weights ranging from 60 to 100 statistical units. Tworegions of behavior are observed.

For t < Tr, the front is discontinuous for reasons discussed above and Nm can beapproximatedby summing average contributions from single chains Vl(t) as,

Nm = n(t)VI(t), (31)where n(t) is the number of chains crossing unit area (or unit length) of the initial interfaceplane. From Table 1, it can be seen that n(t) scales as n(t) = X(t)/M where X(t) is theaverage monomer diffusion distance (equivalent to used in Fig. 8). The contributionto the diffusion front from a single minor chain is given by the square root of the contourlength which is proportional to X(t). Substituting in Eq. 31 we obtain,

Nm= X(t)2/M. (t

17

Fig. 8 shows that the plot of log Nm vs. log X(t) has a slope of 2 for all molecularweights and that at constant X(t), Nm varies approximately as the inverse of M. However,for times less than the reptation time, the diffusion front is not considered to be fractalsince the criterion of self-similarity is not obeyed due to discontinuities in the interfaceplane. This concept may need to be modified when consideration is given to short rangesegmental motion proposed by Zhang and Wool (15). Rouse-like motion of short chainsegments was not considered in this simulation and the results reflect the concentrationprofile for monomers on the primitive path of the reptating chain. The time-dependentscaling law for Nm at t < Tr is seen from Table 1 to be identical to that for bridges, p(t).

At t = Tr, since X.2 = M, Nm(Tr) from Eq. 32 becomes independent of molecularweight. When t > Tr, the number of monomers on the diffusion front is predicted fromSapoval's theory to behave as,

Nm = X 0 -43, (33)

and is shown by the convergence to a slope of 0.43 for all molecular weights in Fig. 8. Thenumber of lattice sites, NL, on the polymer diffusion front was found to behave similarly tothe number of monomers, Nm. A mass-to-radius analysis of the diffusion front geometrygave a fractal dimension of approximately 1.7. These results are in agreement with theatomic diffusion fractal analysis in 2 dimensions. Thus, the diffusion front for polymersbecomes fractal at times greater than the reptation time and at diffusion distances greaterthan the end-to-end vector of the chains.

MICROSTRUCTURAL FRACTURE CRITERIA

Chain Pullout

The Griffith approach to brittle fracture is given by (37)

(6U/6a)6 _ 2F, (34)

where U is the stored strain energy consumed at constant displacement, 6, to advance acrack by the increment, 6a, and create surface energy, 2F6a. The fracture energy, or thecritical strain energy release rate, Gic, is related to F by

Gic = 2F. (35)In principle, if one independently knows the surface energy, F, of a solid one should be

able to predict its fracture energy using Eq. 35. However, for high molecular weightentangled polymers the experimental values are typically of the order GIc == 1000 J/m2 andF = 10- J/m 2. Closer agreement with the Griffith theory is obtained for brittle fracture ofvery low molecular weight unentangled polymers (38, 39).

The Griffith idea has considerable value if one can determine how stored energy isconsumed in forming the fracture surface. To address welding and healing problems astored strain energy approach to fracture was adopted which considers both chain pulloutvia disentanglement and chain fracture mechanisms at the interface. Consider a volumeelement containing a small area of interface as sbown in Fig. 9 subjected to normal stresses,Uij, and shear stresses, rij. The strain energy density, U, of the element is given by,

U = (u2 xx + U2 yy + 2zz)/2E

18

- (axxayy +ayyozz + rxxazz) V/E (36)

+ ([ 2 xy + t2xz +-C2 yz)/2,us,

where E, v and p s are Young's modulus, Poisson's ratio and shear modulus, respectively.

Fig. 9. A segment of a stressed chain at an interface is shown.

We first consider a uniaxial stress field with a = ax and all other stress terms equal tozero. In that case, the strain energy density is

U = 02/2E. (37)We can reasonably assume that the modulus behaves as, (1, 40)

E = tM; (38)

Eoo = M , (39)

such that E can be assumed to remain constant during healing and fracture.

The number of chains per unit volume, Nv, is

Nv = o Na/M, (40)

where o is density and Na is Avogadro's number. The strain energy per chain, Uc, istherefore obtained as,

Uc = U/Nv = a2M/(2E o Na). (41)

The strain energy associated with a segment of chain of length 1, is similarly derived as

Uc t U21. (42)The stored elastic energy can be used to either pull the chain out from the interface orfracture the chain. A fracture criterion for chain pullout can be written as

Uc _> Up (43)

where U p is the energy to pull a chain out of its tube with a force f, and velocity, dl/dt.

19

The pullout force is given by f = u dl/dt, where u is the friction coefficient for the chainsegment of length, 1. The friction coefficient for the segment is related to the monomerfriction coefficient, duo, via/p = pol such that the force may be written as,

f = 1 o 1 dl/dt. (44)The energy required to pull a segment out at constant velocity is determined from

l=L

Up = JUo l(dl/dt) dl, (45)

1=0

as, (41)

up = puo (dl/dt) 12/2, (46)

or

Up = 12.

A similar result is obtained if the chain is pulled out at constant force rather than atconstant velocity, V=dl/dt. Eq. 46 has also been derived by Prentice (42) and Evans (43).

Substituting Eqs. 42 and 46 in Eq. 43, the critical fracture stress for chaindisentanglement (and tack) is obtained as,

o, = (oVEb o Na/Mo) 1/ 2 l(t) 1 / 2 , (47)

or,

u = X(t), (48)

such that

a = vI(t)

where X(t) - vl(t) is the average monomer segment interpenetration distance, Mo is themonomer molecular weight, and b is the bond length. Examining the scaling laws in Table1, the fracture stress or tack in uniaxial tension should behave as,

a- =tl/4 M -1/ 4 , (49)

and the virgin (green) strength as

a, = M 1/ 2 . (50)

20

The velocity dependence, V = dl/dt, of tack and green strength during peel adhesiontests from Eq. 47 should behave as,

o=V 1!2 . (51)

Fracture by the chain pullout mechanism is favored at low molecular weight (smalll(t)), low deformation rates (small V), high temperature (lowp%), short healing times(small l(t)) and plasticizing agents (low uo).

Fracture Mechanics of Welding

The Dugdale model (44) was used as a first approximation to determine the molecularaspects of the fracture mechanics. In this model, shown in Fig. 10, a crack of initial lengthao propagates through a plastic line zone or craze of length rp, ahead of the crack tip. The

CT

t x

Fig.. 10. The l~ydale model for a crack p propagating through a welded interface ofthickness X -1'! is shown. The stress, u, acting on the plastic zone of length ro, draws theinterface into craze-like fibrils of constant draw ratio, \, which break down to tJ'roduce thecrack opening displacement, 6 (R. P. Wool).

plane stress field near the crack for a Cartesian volume element, xyz, and angle a atdistance r is given by Rice (45) as,

= K/2r cos a/2 (1-sin a/2 sin 3a/2) +.....

y= K/2.rr cos a/2 (1 +.sin ./2 sin 3a/2) + .(52)

= Ki/ rrcos.a/2 +......

where KI is the stress intensity factor. The length of the plastic zone is determined by

rp = at/8 Kic2/U~c, (53)where c is the craze or yield stress.

The critical crack opening displacement is given by

6 = KIc2/Urc E, (54)

where E is the tensile modulus.

21

Using the approximation that uc remains constant within the plastic zone, the criticalstrain energy release rate, Gic, is determined by

GIc = Uc6 , (55)

such that the fracture energy is determined as a critical force acting over a critical distance.

Fig. 11 shows the essential features of the Dugdale model for a crack propagatingthrough a line deformation zone in styrene-isoprene-styrene (SIS) block copolymer (46).The microstructure elucidated by Transmission Electron Microscopy (TEM) consists ofstyrene spheres (white) with a diameter of ca 250 A in an isoprene matrix (stained blackwith osmium tetroxide). For the craze zone, r = 3 pm and 6 = 0.2,um. The crazepropagates in the stress field applied normal t9 the craze by incorporating a sjngle styreilesphere into the tip of the zone. As the zone propagates it thickens from 250 A to 2,000 Aby drawing further material into the zone and elongates by extending the material alreadyin the zone. At the crack tip, many styrene spheres have been drawn into the zone anddeformed nonuniformly such that the crack tends to propagate through the center of thezone. Similar mechanisms have been identified for crazes propagating through pureamorphous polystyrene (47, 48). Thus, a critical stress nucleates the line zone at distancerl from the crack tip and the crack opening displacement is determined by the breakdown

the material drawn into the zone.

Fig. 11. (a) Transmission Electronnucrograph of a plastic zone, r =3 pm,in a mechanically stressed Styr'ne-Isoprene-Styrene thin film. The whitespherqs (styrene) have a diameter of-250 A. The number of spheres in thezone increases towards the crack tip(6 = 0.2 pm) due to zone thickening. (b)Shows details at a crack tip, 6 = 1.0 pm,and plastic deformation zone extendinginto the undeformed S-I-S sample.(Dolman, Robertson and Wool).

b

22

To evaluate the molecular aspects of the welding problem we first calculate cc usingthe strain energy approach such that the stored energy per molecule in an xy-plane stressfield is,

Uc = (u2xx/ 2 E + u2yy/ 2E + - 2xy/ 2 )/Nv. (56)

Substituting for the stress terms from Eq. 52 in Eq. 56, Uc is found to be dominated by theuyy term and can be well approximated by

Uc = C2yy l(t), (57)

where l(t) is again the average interpenetration length. Using the same criterion for chainpullout, Eq. 46, and letting uyy = oc at critical conditions, then

1c l(t) 1 / 2, (58)

which is similar to the result obtained for the uniaxial case. For glassy polymers, ac can berelated to the craze stress which differs from the shear yielding stress, ay.

The critical crack opening displacement, 6, is determined by the breakdown of theentanglement network in the deformation zone and the extent to which the zone canthicken as depicted in Fig. 10. During welding, the zone consists of interdiffused shortchain segments mixed with longer chains with nonequilibrium configurations and theentangled structure is complex. The crack opening displacement consists of twocomponents: a component from the virgin material, 6v , and a component from the thediffuse interface, 6i, such that 6 = 6 v + 6i . At low welding strengths the contribution fromthe weaker interface dominates since the energy required to thicken and propagate thezone into the virgin material is too high. The crack opening displacement is thendetermined by the breakdown of the entanglement network in the interface by thefollowing approximation (50),

61/ afl(t) 1/ 2 , (59)

where af is the constant uniaxial draw ratio to tighten the slack between entanglements.

At this point we briefly consider an entanglement model which can be used to visualizethe breakdown process of the deformation zone at the crack tip shown in Fig. 10. Anentangled amorphous linear chain network is shown schematically in Fig. 12. The bridgetheory of connectivity in an amorphous network proposed by Wool (3, 4) requires that thenumber of bridges p, crossing any load bearing plane exceeds the number of chains n,intersecting the plane. In terms of a single chain argument, this implies that each chainmust be long enough to create one link or bridge, i.e., the chain minimally forms one circleor knot with its surroundings as shown in Fig. 12. The critical entanglement molecularweight MC, occurs at p = n and is given by (3, 4)

Mc = 30.89(zb/c)2Mo Cooj (60)

in which z,b,cI M Coo and j are the number of monomers per c-axis length (see examplesbelow), the boniength, the c-axis length, the monomer molecular weight, thecharacteristic ratio and the number of bonds per monomer, respectively. For example, with

I 23

Fig. 12. An entangled network of linear polymer chains is shown. The bold structureillustrates the minimum bridge structure required of each chain to form the network.

polystyrene, b = 1.54 A, c = 6.5 A for an isotactic chain, z = 3 monomers per helicalrepeat distance, M o = 104, Coo = 10, j = 2 c-c bonds per monomer, such that Eq. 60predicts Mc = 32,000. This compares well with the critical entanglement molecular weightfor the cross-overof the zero shear melt viscosity f om Rouse (q = M) to entangledbehavior (q M'r 4 ). For polyethylene, b = 1.54 A, c = 2.55 A, z = 1, M o = 28, Co =6.7, and j = 2 such that M = 4,000. The calculated values compare well with experimentand can be approximated for most vinyl polymers by Mc = 30 Cc, M o.

Applying this model to examine disentanglement as a function of draw ratio, a, thenumber of chains crossing any plane normal to the applied strain increases IsT(a) = anand the number of bridges increases more slowly as p(a) = poa/(a2 + 1/a)'! . At thecritical point of p(a) = n(a), the critical draw ratio is determined by ac2 + 1/ac = 2M/Mcsuch that,

ac = (8/3 M/Mc) 1/ 2 cos{1/3 cos "1 [-1/2(3Mc/2M) 3/ 2]} (61)A useful approximate solution to Eq. 61 at M o Mc gives the critical draw ratio for

disentanglement as

ac = (2M/Mc) 1/ 2 (62)

In a welding interface, the interdiffused contour length provides new entanglements whichdecrease with draw ratio such that a critically connected state exists at,

ac = (21(t)/Lc) 1/ 2 (63)

where Lc is the entanglement contour length corresponding to Mc.

Entanglement models (49, 50) predict that the strain hardening fibril draw ratio isconstant with values of af - 4 which is in agreement with TEM studies of craze fibrils byDonald and Kramer (49). When ac < af, Rouse-like retraction of the stretchedentanglements will relax the contour length such that the critically connected statepredicted by Eq. 63 exists. An instability arises which results in the completion of thefracture process. Substituting for r and 6, the critical strain energy release rate isdetermined by

24

GIc = t 1/ 2 M' 1 / 2; (64)

Goo = M. (M < M*) (65)

The critical stress intensity factor, KIc, is related to the fracture energy via

GIc = KIc2/E, (66)

and is expected to increase with welding time as

Kic = t 1/ 4 M-1/4; (67)

KIc_ = M1/ 2 (68)

If the chains in the deformation zone cannot disentangle completely and bond ruptureoccurs then the scaling laws become more complicated. For welding of glassy polymers,fracture involves a mixture of disentanglement and bond rupture mechanisms. de Gennes(26) has suggested that molecular bridges could control the strength, which is similar to thecrossing density suggested by Prager and Tirrell, (7) and which is similar to the totalnumber of entanglements per chain per unit area suggested by Kausch (52). In that case,the fracture energy is given as

Glc = tl/ M-32 (611

Glcoo = Mo . (70)

The above relations for welding and fracture will be explored in the experimental section.

Stages of Healing

Healing of polymer interfaces has been described by Wool and O'Connor in terms ofseveral stages involving (1), (a) surface rearrangement, (b) surface approach, (c) wetting,(d) diffusion and (e) randomization. Most of the above discussion focussed on theinfluence of diffusion on mechanical properties. However, several other factors can affectthe welding process and are discussed below as the "stages of healing".

(a) Before the surfaces are contacted, one should consider the roughness ortopography of the surface and how it changes with time, temperature, and pressurefollowing contact. In fractured polymers, rearrangement of fibrillar morphology, etc., canaffect the rate of crack healing. Chain end distributions near the surface can change asmolecules diffuse back into the bulk polymer. Spatial changes of the molecular weightdistribution may also occur, e.g., where the low molecular weight species preferentiallymigrate to the surface. Chemical reactions, e.g., oxidation and crosslinking can occur onthe surface and complicate the molecular dynamics of diffusion. Many other processes,e.g., molecular orientation changes, can contribute to the stage of surface rearrangement.Each material and experimental technique usually possesses unique surface rearrangenieitprocesses which may need to be quantified. O'Connor (57) found significant effects ofsurface rearrangement on the healing rate of lightly cross-linked polybutadiene such thatthe fracture energy at constant healing time decreased with increasing surface

2S

rearrangement time (prior to contact). This effect can be explained by the chain endsdiffusing back into the bulk such that they were not as readily available for diffusion duringhealing. Recent SIMS analysis by McGarel and Wool (unpublished) of low molecularweight deuterated polystyrene chains on the surface of high molecular weight polystyrenesupport this concept. T hey found that the low molecular weight species will notpreferentially migrate to the surface but will distribute uniformly in the bulk material.

(b) Surface approach considers time-dependent contact of the different parts of thesurfaces to create the interface. For example, in crack, (1, 18) craze, (53, 54) and void (55,56) healing, contact may be achieved at different locations at different times in theinterface depending on the closure mode (1). For example, slow closure of a doublecantilever beam crack would result in different extents of healing along the closed crack.This stage typically contributes as a boundary value problem to the other stages of wettingand diffu sion.

(c) Wetting can occur in a time-dependent fashion at the interface. For our purposeswe provide a brief phenomenological description of wetting to illustrate potential problemsin evaluating the time-dependence of welding. Fig. 12 shows a schematic region of theplane of contact of a polymer interface (1). Due to surface roughness, etc., good contactand wetting are not achieved instantaneously at all locations. Typically, wetted "pools" arenucleated at random locations at the interface and propagate radially until coalescence andcomplete wetting are obtained. This problem has been treated phenomenologically as atwo-dimensional nucleation and growth process such that the fractional weLted area, 4)(t),is given as (1),

(I)(t) = 1 - exp(-kt m ) (71)

where k and m are constants depending on the nucleation function and radial spreadingrates.

Contact theories proposed by Anand (72) and others suggest that complete strengthmay be obtained when the interface has wetted at (D = 1. Others argue that interdiffusionis necessary for strength development. The time dependence of viscous flow to promotecontact and that of interdiffusion may be comparable since they are subject to the samemolecular dynamic processes. We will demonstrate in later sections using both tackexperiments and incompatible interface weld strength data that diffusion plays a veryimportant role.

(d) The diffusion -tage has been discussed above with respect to the instantaneou.wetting condition. However, in the presence of a time dependent wet-ing function, Eq. 71.we see from Fig. 13 that diffusion will have progressed to different extents in differentareas of the interface. If the intrinsic diffusion function, H(t) as given by Eq. 23, does notchange its nature with time due to the other stages, then the net diffusion, H'(t) can beexpressed as the convolution product,

H'(t) = (t-r) d(l)(T)/dr dr, (72)

where r is a "dummy" variable on the time axis. The convolution process for typical (1)(t)functions may mask the time-dependence of the intrinsic diffusion function and related

26

mechanical properties. This part of the problem can be solved mathematically by lettingthe wetting function be a Dirac delta function,

d ()(t) = (5 (r), (73)dt

such that Eq. 72 reduces to H'(t) - 1-1(t). This can be attempted experimentally byobtaining inotantancous wettilg of atomically smooth surfaces under moderate contactpressure at temperatures above T However, we have found that the wetting problem canresult in diffictty with the analysi of most short time welding data.

0

iI

Fig. 13. A schematic view of the stages of healing in an interface. Contacted regions ofradius r grow and coalesce. Interdiffusion occurs only in the wetted regions while surfacerearrangement occurs in the non-wetted areas. (Wool and O'Connor)

(e) The randomization stage refers to the equilibriation of the nonequilibriumconformations of the chains near the surfaces and in the case of crack healing andprocessing, the restoration of the molecular weight distribution and rai.om orientation ofchain segments near the interface. The conformational relax.,tion is of particularimportance in the strength development at incompatible interfaces.

The stages of crack healing can have interactive time-dependent functions such that thewelding and tack problems can consist of processes involving five-way interconvolutedfunctions resulting in mechanical properties whose time dependence may not be readilyinterpretable. Thus, great care must be taken in conducting welding experiments which aredesigned to critically explore molecular theories of strength development.

HEALING EXPERIMENTS

Tack and Green Strength

The critical experiment is~o s s tl the tack or stress at fracture of uncured linearelastomers bfehaves as a = t 7 M - / V and that the green or virgin strength behaves asgoo-- (MV) /-. In addition, the self-diffusion coefficient should b,- measurable as D =A/M 2 where A is a constant derivable from mechanical data. The concurrence of

27

predictions derives from the molecular dynamics analysis of tack and greca strength. Thesepredictions apply to all amorphous linear polymers whose chain configurations can bedescribed by Gaussian statistics and whose fracture behavior is dominated by chaindisentanglement mechanisms.

Fig. 14 shows tack data obtained by Skewis (61) for several polymer-polymer pairswhere we ve replotted the tack (units of force applied to a cross-sectonal area of 0.4cm2 ) vs. t/. The original data were nonlinear when plotted on a t VAe to investigatediffusion mechani !s. However, the fracture energy behaves as GI = t / ' while the tackbehaves as a = t a/'s evidenced by the linear plot in Fig. 14. The SBR/Butyl pair areincompatible and the long tim, quilibrium strength is considerably weaker than either ofthe symmetric pairs. Similar c /4 results for tack have been reported by Wool andO'Connor (1, 40) for polybutadiene, and by Voyutskii (11) for polyisobutylene.

CONTACT TIME (SEC)

700 1.0 16 81 26

600 o SBR/SBR*BUTYL/BUTYL

< oSBR/BUTYLASBR/GLASS

40

~00

Z 200

Y~r100

0 1.0 2_0 30 4.0 50

(CONTACT TIME) (SEC) t/4

Fig. 14. The tack or breaking load vs. t 1/ 4 for several polymer-polymer uncured pairs asinvestigated by Skewis (61). lack measurements were done with a contact load of 1000 gand a contact area of 0.40 cm . The viscosity-average molecular weight, Mv, of the SBRwas 260,000 and 225,000 for the butyl rubber.

The molecular weight dependence of tack and green strength was investigated byForbes and McLeod (62) for fractionated samples of Hevea. Their results are shown inFig. 15 in which the upperline represents the green strength and the bottom line representsthe tack stress evaluated at a constant contact time of t, = 30 sec for each molecularweight. The green strength curve was obtained theoretically using (1)

aoo = k1(M 1/ 2 - Mi1/ 2 ), (74)

where k1 = 993 f/1jM 1/ 2 and M. 1 / 2 = 284.1 is the intercept on the a.0 = 0 axis of theplot of a,, vs. M'/ 1 . The curve through the tack data in Fig. 14 was determined by theoryas

(I = ao + aM " 1/ 4 , (75)

where a = 5.29 MPa M1 / 4 and ao -- 80.5x103 Pa s constant dependent on the initialwetting conditions of the interface. When a = k2 tf /i as in Fig. 14, the constant, k2 , isrelated to the constant, a, in Eq. 75 by

28

k2 = a/(M1 / 4 tcl/ 4 ), (76)

where in this case tc = 30 sec. Considering the difficulties in performing such experiments,the agreement between theory and experiment in Fig. 15 is satisfactory. If the strength iscontrolled by bridges, then a - M -3 /'at constant tc and u(o = Mo. These predictions areinconsistent with the data in Fig. 15. It has been suggested that the tack stres isindependent of molecular weight but in fact it behaves approximately as M'/4 in closeagreement with disentanglement theories. This is a weak molecular weight dependencebut related mechanical properties such as fracture ,, rk, 3k, should behave with astronger molecular weight dependence, as GIc = t /'M- ,

In Fig. 15 the green strength is seen to rise steadily up to M = 1.5 x 106 at which pointit remains fairly constant and bond rupture is expected to dominate the fracture mechanismby regulating the extent of disentanglement. Given sufficient time, the tack stress willincrease to the green strength value by continued diffusion. Using tracer diffusionmethod.,,kewis (63) measured the self-diffusion coefficient of natural rubber at 25C as D= 3x10- cm 2/sec using samples with a viscosity-average molecular weight of M v =234,000. The polydispersity of his samples was not known. The self-diffusion coefficientfrom healing data is given by (1-3)

D = (k2 /k 1 )4 b2 Co0/6MMo, (77)

where C. is the characteristic ratio for the dimensions of a random-coil chain. Letting M= 234,000, M = 68 for polyisoprene b =,4.05 A from the c-axis of the cis-14-polyiso-prene unit cei, and k2 = 0.103 MPa/sec 1 / from Eq. 7. we obtain D = 10-14 cm2/secwhich is of the same order of magnitude as D = 3 x 10-N cm 2/sec obtained by Skewis.

250[

NATURAL RUBBER

200

50"I

1) 0. . . . .

-I. . .-. . . -' . . I

MOLECULAR WEIGHT X 10-6

Fig. 15. Tack (circles) and green strength (triangles) as a function of viscosity averagemolecular weight for fractionated samples of natural rubber (Forbes and McLeod) (62).The solid line for green strength was theoretically obtained using Eq. 72 and the dashedline for tack using Eq. 73. The green strength was evaluated at a umiaxial test speed of26.67 cm/min at 25C, and the tack was evaluated at a constant contact time of 30 sec foreach sample. Filled and unfilled data points refer to unmillled and milled natural rubber,respectively.

The reptation time, Tr , is obtained from the self-diffusion coefficient as

Tr = R2/(3;r2D), (78)

where R 2 is the end-to-end vector given by R 2 = Mj/M o C.o b2. For natural rubber thehealing time is approximated by

29

Tr = 2.48 x 10- 15 M3 sec. (79)

When M = 234,000, Tr = 32 sec and in Fig. 15, this material should be in the green state attc = 30 sec as observed. The healing time required for the samples with M = 1,000,000 isabout 40 min. These results differ with those of Roland and Bohm (69) who found that thetime required to achieve maximum autohesive strength of polybutadiene was orders ofmagnitude longer than the time required for the chains to diffuse a distance approximatelyequal to the end-to-end vector, R. Chain branching and nonuniform wetting at theinterface may have contributed to this difference.

Stacer and Schreuder-Stacer (95) investigated the time dependence of alohesion inpolyisobutylene. Molecular weights of their samples ranged from 1.5-21 x 10-' with poly-dispersities of 1.1 to 3.6. T-peel test configurations were used to evaluate the peel energy,G, as a function of time, molecular weight, temrature and pressure. Fig. 16 shows a plotof log G vs log t/aT for PIB with M = 1.5 x 10'. The contact time was reduced withrespect to the time-temperature shit factor, aT , to create a master plot from data obtained

--"-0N 3- ' q .

CD Cy 1/2

, / ...

-2 0 2 4 6LOG tc/a T (S)

Fig. 16. Comparison of the predictions of several theoretical models with autohesion datafor PIB (Stacer and Schreuder-Stacer).

at different tempera Tpys. Several theories were examined. The scaling law for peelenergy is G - (t/M) / as given by Wool, et al., in Eq. 64, predicts a slope of 1/2 as shownin Fig. 16. They conclude that the 1/2 power law slope is applicable to describe limitedregions of the data but does not provide an overall description of the autohesion curve.The time to achieve equilibrium strength (healing time) to,, was predicted by Wool (3) as,

too = C.o b2 M3 / (6AMo) (80)

where A is the constant in the self diffusion coefficient relation, D = A/M2. This relationwas found to be in excellent agreement with the PIB autohesion data. The molecillaweight dependence of healing was not properly analyzed in this work since the M/"dependence of the healing rate was incorrectly compared to the green strength energy, G .

The monodisperse and polydisperse chain interdiffusion theories of Prager and Tirrellare compared with experiment in Fig. 16. This model determines the number of effectivecrossings per unit area where an effective crossing involves a minimum interpenetrationdistance related to the entanglement molecular weight spacing which allows a chainsegment to participate in energy dissipative processes. The agreement is good for themonodisperse case and the polydisperse model reasonably described similar studies. Bothmodels predict a slower rate of healing (about 1/2 time decade) compared to experiment.

30

Fig. 16 also compares a wetting theory of Korenevskaya, et al. (96), expressed as a firstorder kinetic process in terms of the fractional peel energy G = G(t)/G , as

G + In (1-G) = - P t/u

where P is the applied pressure and/a is the zero-shear viscosity. This relation providedexcellent agreement with the data. Deviations to significantly lower GIc values wereobserved at short times with the high molecular weight PIB samples.

Since the diffusion controlled healing times are comparable to characteristic relaxationtimes of viscosity, this work cannot readily distinguish between wetting and diffusiontheories. Studies by Wool and O'Connor (21, 57) of tack and healing in hydroxy terminatedpolybutadiene (HTPB) indicated that the mechanical property recovery due to wettingoccurred in a few minutes and was a small fraction of G a, while interdiffusion of thepartially cross-linked chains took several weeks during which the majority of the fractureenergy was recovered. The separation of the relaxation times for wetting and diffusion inthat case support the diffusion model.

A more convincing case for the diffusion model is obtained from studies ofincompatible amorphous polymer interfaccs such as PS/PMMA. At long contact times,complete wetting or contact has been achieved but the incompatibility only allows limitedinterdiffusion with with correspondingly low fracture energy. The observed fractureenergies of incompatible interfaces by the Urbana group are consistent with the diffusionmodel such that the fracture energy increases as the compatibility of the polymer pairs andinterdiffusion increases at constant contact area. A possible flaw in this argument is thatthe incompatibility influences chemical interactions, e.g., acid-base, at the contact planewhich would affect the wetting theory. However, the contact plane no longer exists as suchdue to the limited diffusion which has occurred.

Pressure affects diffusion by decreasing the free volume which slows the hoppingprocess necessary to achieve Brownian motion and subsequently decreases the self-diffusion coefficient. This effect is more pronounced near the glass transition temperatureand is important in polymer melt processing where large hydrostatic pressures can beencountered. It is not very important in normal tack experiments where the contactpressures are usually much less than a kilobar. However, pressure affects the wetting stageby promoting better contact. Thus, tack measurements should be dependent on pressure tosome degree while wetting is occurring but should be largely independent of pressurewhen interdiffusion is occurring. Expressions for the pressure dependence of Tr and Dhave been given (1, 3).

The effect of strain rate and peeling velocity on tack has been examined by manyinvestigators. Fig. 17 shows data obtained by Hamed (64) for the cohesive strength of anSBR elastomer (FRS-Ifl6)as a function of peel rate using a T-peel test configuration. Theprediction that u = V , is observed to be in agreement with the high temperature data(where chain pullout is expected to dominate) as judged by the slope of 1/2 for the plot oflog r vs. log rate. As the temperature approaches T , -50'C, chain fracture begins tocontribute to the defofpmtion mechanism and the /2 behavior is lost as predicted. Theprediction that a V/2 is also supported by data of Tsuji, et al. (65) for T-peel tests ofpolyisobutylene and by data of Bhowmick, et al. (66), for adhesive tack and green strengthof EIjM rubber. The dependence of the fracture energy, G, on the rate of peel is also G= V/'P since the extent of disentanglement and not the rate determines the crack openingdisplacement for the chain pullout mechanism.

4 - _. 4

-35oC 31

1.2 -

z 1.0-4'C

F-(9 08-zIi

"n 0.6El>(n 23C/tJi 0.4-

0o

o0 0.2-//

0-

-0.2-

-04 I V

06 1.0 1.4 1.8 2.2 2.6 3.0

LOG RATE (mm/min)

Fig. 17. Cohesive tear strength of SBR as a function of peeling rate at several constanttemperatures (Hamed and Shieh) (64). The dashed line represents the theoretical slope of1/2 and was added for comparison purposes. The SBR was a cold emulsion styrene-butadiene random copolymer containing 23% bound styrene and had a Mooney viscosity(ML-4, 100'C) of 40.

For peel adhesion, the pullout mechanism predicts the fracture energy to behavt as

G = (t V/M)1 / 2; (81)

G = MV 1/ 2 . (82)

Several other theories of tack and adhesion have been presented. Bister, et al. (67),predict that the peel energy behaves as

G = M2 / 3 (Dt) 1/ 2 . (83)

Since D = M- 2 and T = M3, then Eq. 82 predicts that G = t1/2 M -5 / 3 and G_ = M- 1/ 6 .However, this molecular weight dependence cannot be supported by data reported here orelsewhere. Most theories predict the t/ dependence but as seen from Table 1, this is nota unique function.

Wu, et al. (68) predict that the adhesive strength is deter~ed b n(t)X(t) whichbehaves in an identical manner to bridges (Table 1) as G = t /- M and G. = Mo .The molecular weight dependence of these relations is not supported by experiments.However, Wu, et al., also suggest that the number of chains, n(t), sauiates fluickly and thatG depends on center-of-mass motion over larger distances as G -= t 7 M- . We disagreewith the latter suggestion since n(t) increases simultaneously with the strength for times t M*, as can be deduced from Fig. 26. These resuits are ofimportance for composite lamination of thermoplastic matrices. We propose furtherstudies of fatigue-healing problems.

Fatigue crack healing is also an important concept for fiber filled composites.Klosterman and Wool (101) found that damage involving fiber-matrix failure and matrixcracking in glass fiber filled thermoplastics could be healed at temperatures above T,. Asa result, the FCP rate decreased with increasing healing time in the damage zone un il thevirgin state FCP rate was obtained. It was also found that complete crack healing could beobtained with highly cross-linked epoxies. These studies suggest that the lifetime ofcomplex composites in practice could be considerably increased by periodic healingtreatments. The possibility also exists that specific microwave and other treatments couldbe used to excite healing processes in specific regions of the composite.

40

I c- -- - - --0 - - - - - - -T

z

toi-ci

T -

-o 117" 0o E O_3-

U--

'A

o 5'0

0 09

1 10 101 105 I 5 2Welding Time (mil) 105MOLECULAR WEIGHT, MwxlO

4

Fig. 25. Fatigue crack propagation Fig. 26. Fatigue crack propagation ratesrate of polystyrene vs. welding time at vs molecular weight of PVC (Rimnac, et al.).contam G = 240 J/m2. Mn = 133,000 The solid line is given by gsentang~erentand Mw/!in = 2.3. (Yuan and Wool). theory by daidn = a/ -'4JL- Mcr-J/) where

a = 4.5 x 10' mm M-'- cycle and Mc' -60,000 is the molecular weight at whicbhcritical crack propagation occurs at K = 0.7MPa Vm.

Incompatible Amorphous Interfaces

With immiscible, incompatible, amorphous polymers the equilibrium structure of theinterface is determined thermodynamically by the balance of (1) the decrease of freeenergy due to entropy relaxation of the surface chain configurations and (2) the poji 'ywenthalpy of mixing produced by limited diffusion to a distance doo. Since do, = X- /according to Helfand, , al. (24, 86) and the Flory-Huggins interaction parameter, X.behaves with temperature approximately as X = l/T, we expect for fiacture dominated bychain pullout that Gic lo do,2 and that the equilibrium strength behaves with weldingtemperature as, (22, 77)

Gc * T. (95)

The equilibrium fracure energy for several incompatible interfaces was obtained byFoster, Willett, et al. using wedge cleavage methods (77, 87. 102). These includedPS/PMMA, PSAN/PMMA, PC/PSAN. Gic was found to increas - with temperature inreasonable agreement with Eq. 95 for PSAN/PMMA and PC/PSAN interfaces but wasfairly independent of temperature for PS/PMMA up to 170 C.. Typical measured fractureenergies of order 40-200 J/m 2 were greater than either the initial wetted energy (about 5J/m2) or the average surface energy, F < 1.0 J/m2, indicating that limited diffusion hadtaken place. The dynamics of welding incompatible, amorphous interfaces was found to becomplex and will not be presented.

41

The equilibrium strength of incompatible interfaces occurs with full contact of thesurfaces and appears to be dependent on the extent of the limited interdiffusion which is afunction of temperature, molecular weight and chemical compatibility. For example, inFig. 14, the SBR/Butyl interface in the autohesion experiment is incompatible and lowstrength is achieved compared to the symmetric SBR/SBR and Butyl/Butyl interfaces eventhough good contact has been achieved at very long times. This observation stronglysupports the diffusion mechanism of strength development at amorphous polymerinterfaces.

The magnitude of the equilibrium interpenetration distance, doc, can be approximatedfrom the mechanical data using the following scaling relations,

[doo/SA]P = GIc(A/B)/GIc(A/A) (96)

or,

[dc/SA] = o(A-/B)/u(A/A) (97)

where SA is the radius of gyration of the pure A-component, GIc(A/B) and U(A/B) are theequilibrium fracture properties of the incompatible pair and GIc(A/A) and u(A/A) are thevirgin state fracture properties of the A component. It is assumed that the pure polymers Aand B have the same virgin state mechanical properties and molecular weights. Forexample, the butyl elastomgr in Fig. 14 has a viscosity average molecular weight, Mv225,000 such that S - 200 A. If u(A/B)/ur(A/A) = 100/400, then from Eq. 97, we obtaindc z 50..

For PS/PMMA interfaces, Foster and Wool (87), using wedge cleavage methodsobtained constant values of GIc = 45 J/m2 for welding at temperatures bqtween 100 and170'C. If we assume that for polystyrene with M = 250,000 and S = 138 A that GIc(A/A)= 1000 J/m 2, as shown in Fig. 21, then from Eq. 96, doo = 29 A. The Flory-Hggginsinteraction parameter X, is related to cc by X 0.66 (b/doo) 2, where b = 6 A is thestatistical segment length. If dcc = 29 A, then X 0.028 for the PS/PMMA interface. Thetemperature independence of the fracture energy for PS/PMMA interfaces are consistentwith the very weak temperature dependence of X measured by Russell, et al. using neutronscattering techniques (103).

Incompatible Crystallizable Interfaces

Strength development at incompatible, crystallizable interfaces such as polyethylenewith polypropylene, PE/PP, can occur by different mechanisms than those discussed above.In the melt, limited diffusion to a depth, d.c, first occurs. When the interface cools, crystal-lization occurs first in the PP side due to the difference in melting points. Random nuclea-tion of spherulites near the interface coupled with the volume contraction due to crystal-lization breaks up the interface. PE melt riverlets are drawn into the PP side whichsubsequently crystallize and effectively mechanically interlock the interface. This mech-anism has been discussed by Galeski (88, 89) in terms of "local crystallization" creating"influxes" across the interface and has been investigated by Yuan and Wool (77, 90).

Fig. 27 shows a PE/PP interface during fracture by wedge cleavage methods. Theinterface was crystallized in a manner to optimize the mechanical interlocking effect. Thefibrillar structures in the fractured interface are due to plastic deformation of the PEinfluxes. The fracture stress was measured as a -u 10 MPa which is more than half thevirgin strength of PE. In the absence of influxes, the interface is extremely brittle with a

42

1 MPa. Fig. 28 shows a magnified view of the PP side obtained by SEM (90). The PEfibrillar remnants are clearly seen in the interstices of the PP spherulites. In addition to theinfluxes, PP spherulites which nucleate on the interface planc entrap PE melt on a finerscale between the crystalline lamellar structures as seen by the "white decoration" ofplastically deformed PE on several PP spherulites.

Fig. 27. Fracture of a PP/LLDPE incompatible semi-crystalline interface. The fibrils onthe PE top surface are due to pullout of PE material which was incorporated into the PPside during crystallization (Yuan and Wool).

aFig. 28. (a) Electron micrograph of a PE fracture surface from a PP/LDPE interface.Plastically deformed PE fibrils are observed in addition to circular imprints of PPspherulites on the PE side. (b) PP fracture surface from a PP/LDPE interface shows afractured PE fibril remnant and PP spherulItes (Yuan and Wool).

Thus, for incompatible, crystallizable interface, while melt diffusion produces anequilibrium interface of thickness 50 A, the localized crystallization mechanism producesinfluxes to depths of several microns which impart significant strength to the interface.Delicate control of the processing history is necessary to optimize this effect as it is easy tomake a weak interface with incompatible polymers. Methods of optimizing the strengthhave been discussed (90). The same mechanism also exists at the interface betweensymmetric crystallizable interfaces such as PE/PE welding but plays a secondary role todiffusion and homogeneous crystallization.

43

Lap Shear Welding

A lap shear method as shown in Fig. 29 was used to study strength development duringweldina of PS interfaces by Kline an Wool (91). TIhe surfaces had previously not been incontact and care was taken to ensure rapid wetting of the interface. Lap shear sampleswere welded for a given time at constant temperatures above T and fractured at roomtemperature. Fig. 30 shows a plot of the (average of 15 sample shear failure stress, rfvtime to the fourth power at each constant temperature. The linear response of 1f with tis seen at each temperature and provides further support for diffusion controlled strengthat polymer-polymer interfaces.

1.7mm

3.2 mm

5mm -

31.6 mm

Fig. 29. Lap shear joint method used to test weld strength of polymers (Kline and Wool).

The change in slope with temperature was found to be describable by the William-Landel-Ferry (92) theory of thermal activation near T . At T = 113.5C, the activationenergy, Ea = 93.2 kcal/mole is predicted from a WLIanalysis using the parameters for PS,c1 = 13.7, c = 50 and T = 100C, which compares with E = 96.1 kcal/mole obtainedfrom a plot of the superpsition shift factor vs. 1/T in Fig. 30.

The time to achieve complete healing, Th, can be estimated from the upper plateau idFig. 30. At 391.3 0K (1 18.1C), Th = 256 min for the polydisperse PS samples with Mn =142,000 and Mw = 262,000. This time can be compared with related times measured byother techniques. Lee and Wool, (14) using FTIR dichroism techniques, measured therelaxation time, Tr, of uniaxially oriented monodisperse PS with Mn = 233,000 as Tr = 215min. Kramer, et al. (93)ffport a self-diffusion coefficient for monodisperse PS with Mn =255,000 as D = 5.8 x 10 cm2/sec at 1250C. Shifting to 118C using the relation, (93)

log D/T = A - B/(T-T.), (98)

4416 81 256 62! 1296 240

QT. 3888 0

T.38Z 38 1K500

~250

0 2 3 4 5 6 7

t min,

Fig. 30. Shear stress vs. t1 / 4 for lap welding of polystyrene at several temperatures (Klineand Wool).

where B = 710, T. = 49'C and A = -9.49, then Dj OC = 6.42 x 10-18 cm 2/sec. UsingEq. 76, the time required for the center-of-mass to diffuse a distance equal to the end-to-end vector is obtained as Tr = 1000 min which is about 4 times longer than the timerequired to achieve complete strength of the lap shear joint with Mw = 262,000. On theother hand, using Tr = M3 and D = M-2, the relaxation time for the chains with Mn =143,000 at 118C is about 180 min which is in close agreement with the lap shear result.Because of the ramified nature of polymer interfaces with holes and statistical irregularitiesas shown in Fig. 7, the mechanical healing times are expected to be a litt&, ionger (but ofthe same order of magnitude) than the relaxation times determined from moleculardynamics and diffusion studies. It should be noted that when evaluating healing times fromthe reptation theory that at t = T the center-of-mass of chains in the bulk diffuses adistance related to the end-to-end vector (Eq. 76), while the average monomer interpene-tration distance at the polymer interface is equivalent to the radius of gyration (Eq. 17).

POLYMER PROCESSING WELD LINES

Compression Molding

As a final example of welding we consider the compression molding of resin pelletswhere the interfaces and weld lines form when the pellet surfaces contact in the mold asshown in Fig. 31. With increasing time and pressure, the interfaces wet, diffusion occursand the strength of the sample increases to its virgin strength provided that sufficient timefor diffusion is allowed.

IN

TIP, t

Fig. 31. Schematic of powder/pellet interface welding during polymer melt processing.With time, temperature and pressure, the pellet interfaces heal to form the plastic product.

Wool and O'Connor (1) studied the time-dependence of compression molding using PSpellets of the same molecular weight as described above in the lap shear experiments. PSplates, 152 by 152 mm, were compression molded in a Carver Press using a window frame3.18 mm thick. Each plate was molded at 127 0C 60C, with pressures of 5.5 MPa (800 psi)for varying processing times, to . The plate was withdrawn from the mold, quenched, cutinto tensile "dogbone" samplepand fractured at room temperature in uniaxial tension.Weak interfaces within the sample provided a source of crack initiation. Fig. 32 shows the

45

fracture stress (average of 6 4amples) plotted vs. the fourth power of the processing time.The prediction of a(t) = t1 / is again noted to be satisfactory despite the crudeness of theexperiment. The processing time to ieach the virgin state near u. = 41.4 MPa (6,000 psi)was between 10 and 20 min judging by the saturation of the strength at longer times. UsingKramer's diffusion data at 125C, t~ie reptation time for pellets with Mn. = 143,000 is about20 min which is in reasonable agreement with the observed processing time.

v) 3uJ

T,= 127 6 0C

P= 800 psi

LL AVERAGE OF 6 SAMPLE--

PROCESSING TIME (tp/sEC)V

Fig. 32. Fracture stress vs. processing time (t/ 4 ) for compression molding of polystyrenepellets. Dogbone samples were prepared from compression molded plates (Wool andO'Connor).

The molecular weight dependence of the virgin strength, a., of compression moldedPS pellets has been determined by McCormick, et a. g4) using similar sample preparationand fracture conditions. Fig. 33 (1) shows a.. vs. M ', for monodisperse molecular weightPS using data from reference 94. The data are described by

aoo = 0.23(M 1/ 2 - Mi 1/ 2 ) MPa, (99)where the intercept at u = 0 is NrM i = 245. The strength is seen to increase linearly inaccordance with virgin state predictions up to M - 160,000 after which it decreases slightlywith increasing M. The data was obtained from samples compression molded at a constanttime of 1 min at 170C for all materials. We have suggested that under the processingconditions used that samples with M < 160,000 had reached their virgin state at t = 1 minbut that samples with M > 160,000 were not completely lhealed at 1 min and the fracturestress should decrease as observed according to a M- 1/ . The reptation time for M =160,000 is about 1 sec at 170C and the time of 1 min used in this experiment presumablyincludes warm up time in the mold in addition to diffusion times. However, the maximumin strength with increasing M at constant contact time is expected and is similar to the tackand green strength data presented in Fig. 15.

Strength development at internal weldlines in injection molded specimens are expectedto behave similarly although some complications are expected with interfaces involvingoriented molecules at the weldline. However, it is interesting to note that orientationrelaxation occurs at about the same rate as normal diffusion (14). Orientation relaxationmay contribute to interdiffusion at the weldline in a similar manner as for unorientedsurfaces but problems are anticipated with "barrier" effects produced by oriented layerswhich could result in anisotropic diffusion rates.

8046

70-('_

- 60-

XU

b" 50-

--

(9 40-Z1,J

H 30-U)

-J 20-

C0

Z

I 2 3 4 5 6

(MOLECULAR WEIGHT, M)2 x 102

Fig. 33. Tensile strength vs. square root molecular weight of compression moldedpolystyrene (pellets). Molding occurred at 170'C for 1 minute. Monodisperse molecularweights pellets were used. Data of McCormick, et al.

Relation to Vibration Welding

Vibrational welds can be affected in thermoplastics over a frequency range 25-400 Hz,as reviewed by Stokes (104-107). Typical welding pressures are 130-2000 psi (1-14 MPa)with weld amplitudes of 0.3 to 1.6 mm. The welding process can be divided into fourphases which are independent of the thermoplastic as follows. In Phase 1, the weldinterface is heated by Coulombic friction which ends when the interface begins to melt.The penetration, which is the moving together of the separate pieces due to lateral flow outof the interface, is essentially zero during this phase. With continued energy input, theinterface begins to melt and flow and penetration commences in Phase 2 up to a steadystate lateral flow. Phase 3 represents the steady state flow co